What is semi-conductor ? Band diagrams : metal conductorsinsulators Forbidden Allowed semiconductors Forbidden Allowed Forbidden Allowed Forbidden Allowed With very small energy, electrons can overcome the forbidden band. EFEF
Energy Band of a semiconductor Schematic energy band diagram : E Conduction band Valence band Band gap conduction electron hole
Elemental Semiconductors In the periodic table, Semimetal : conduction and valence bands are slightly over ｌ aped. As (semimetal) ~ 10 20 cm -3 Sb (semimetal) ~ 10 19 cm -3 C (semimetal) ~ 10 18 cm -3 Bi (semimetal) ~ 10 17 cm -3 Carrier density : Cu (metal) ~ 10 23 cm -3 Ge (semiconductor) ~ 10 13 cm -3
Si Substrate Manufacturing Czochralski process : * http://www.allaboutcircuits.com/vol_3/chpt_2/12.html; Silicon is the second most common element in the Earth crust. ** http://www.homepower.com/articles/solar-electricity/equipment-products/peek-inside-pv A common form is Silicon dioxide, SiO 2 (Silica). A Si single-crystal with a desired orientation is used. The Si crystal is lifted at a certain rotation speed from melt Si pot.
Fabrication of a Si-Based Integrated Circuit Czochralski method : Si purity (99.999999999 %) * http://www.wikipedia.org/
Shockley Model Contributions for electrical transport : E Conduction band Valence band Band gap conduction electron (number density : n) positive hole (number density : p) Ambipolar conduction Intrinsic semiconductor * http://www.wikipedia.org/
Carrier Number Density of an Intrinsic Semiconductor Carrier number density is defined as Here, the Fermi distribution function is For the carriers like free electrons with m *, the density of states is For electrons with effective mass m e *, g ( E ) in the conduction band is written with respect to the energy level E C, * H. Ibach and H. Lüth, Solid-State Physics (Springer, Berlin, 2003). For holes with effective mass m p *, g ( E ) in the valence band is written with respect to the energy level E V = 0,
Carrier Number Density of an Intrinsic Semiconductor (Cont'd) f p ( E ) for holes equals to the numbers of unoccupied states by electrons : n is an integral in the conduction band from the bottom E C to top E ct : p is an integral in the valence band from the bottom -E Vb to top 0 : Here, E C (= E g = E C - E V ) >> k B T E - E F E C /2 for E C E E ct (E F ~ E C /2) Similarly, E C >> k B T -(E - E F ) E C /2 for E Vb E 0
Carrier Number Density of an Intrinsic Semiconductor (Cont'd) For E - E F > 3k B T, and hence E Ct ∞ Similarly, and hence E Vb -∞ As a result,
Fermi Level of an Intrinsic Semiconductor For an intrinsic semiconductor, Assuming, m e * = m p * = m * np product is calculated to be constant for small n i can be applied for an extrinsic (impurity) semiconductor
Typical Bandgaps Bandgaps between the conduction and valence bands : Bandgap E g [eV] Resistivity [ cm] Ge0.660.5 Si1.112.3 × 10 3 GaAs1.43~ 10 3 C (diamond)6 ~ 7× 10 12 Eg ∝ Eg ∝ Semiconductors : E g ~ 0.1 ~3.0 eV
Typical Bandgap Bandgaps between the conduction and valence bands : * http://fhirose.yz.yamagata-u.ac.jp/text/kiso1.pdf Vacuum level Electron affinity Work function Ionisation energy Electron / hole transport under a bias : http://kccn.konan-u.ac.jp/physics/semiconductor/diagram/a05.html
Intrinsic Semiconductors Band structures : * http://hooktail.sub.jp/solid/shino-PNI-typeSemiconductor-upper/ Energy Probability Some electrons Some holes
Extrinsic Semiconductors p-type band structures : n-type band structures : * http://hooktail.sub.jp/solid/shino-PNI-typeSemiconductor-upper/
Fabrication of Doped Semiconductor Ion implantation : Typical acceleration energy : 10 ~ 500 keV. Annealing required to activate injected ions as donors / acceptors. * http://www.wikipedia.org/
Fabrication of p-n Junctions 1 Alloy type or fused junction diodes : * http://www.circuitstoday.com/semiconductor-diode-fabrication-types
Fabrication of p-n Junctions 3 Epitaxial growth or planar diffused diodes : * http://www.circuitstoday.com/semiconductor-diode-fabrication-types; epi = upon + taxis = arrangement. ** http://www.allaboutcircuits.com/vol_3/chpt_2/12.html
Fabrication of p-n Junctions 4 Point contact diodes : * http://www.circuitstoday.com/semiconductor-diode-fabrication-types Bonded by radio frequency heating.
Intrinsic Semiconductors * http://chemwiki.ucdavis.edu/u_Materials/Semiconductors/Intrinsic_Semiconductors/Intrinsic_Semiconductors Band structures : N V and N C : carrier densities of the valence and conduction bands ECEC EVEV (n i : intrinsic carrier density) Fermi level :
Exercise 1 Find the probability of occupation of a level of 0.05 eV above the conduction band edge of a Silicon device if the Fermi level is 0.7 eV above the valence band edge. Assume the bandgap (E g ) of Silicon is 1.1 eV and the effective mass of electron in Silicon is 0.40 (0.91 10 -30 kg). The Boltzmann constant (k B ) is 1.4 10 -23 J/K, the Planck constant is 6.6 10 -34 Js and the temperature is 300K. Use the conversion ratio: 1 eV = 1.6 10 -19 J.